1 / 31

310 likes | 419 Views

Chapter 3. Carrier Action. Carrier Action. Three primary types of carrier action occur inside a semiconductor: Drift : charged particle motion in response to an applied electric field. Diffusion : charged particle motion due to concentration gradient or temperature gradient.

Download Presentation
## Carrier Action

**An Image/Link below is provided (as is) to download presentation**
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.
Content is provided to you AS IS for your information and personal use only.
Download presentation by click this link.
While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
During download, if you can't get a presentation, the file might be deleted by the publisher.

E N D

**Chapter 3**Carrier Action Carrier Action • Three primary types of carrier action occur inside a semiconductor: • Drift: charged particle motion in response to an applied electric field. • Diffusion: charged particle motion due to concentration gradient or temperature gradient. • Recombination-Generation:a process where charge carriers (electrons and holes) are annihilated (destroyed) and created.**Chapter 3**Carrier Action 2 3 1 electron 4 5 Carrier Scattering • Mobile electrons and atoms in the Si lattice are always in random thermal motion. • Electrons make frequent collisions with the vibrating atoms. • “Lattice scattering” or “phonon scattering” increases with increasing temperature. • Average velocity of thermal motion for electrons: ~1/1000 x speed of light at 300 K (even under equilibrium conditions). • Other scattering mechanisms: • Deflection by ionized impurity atoms. • Deflection due to Coulombic force between carriers or “carrier-carrier scattering.” • Only significant at high carrier concentrations. • The net current in any direction is zero, if no electric field is applied.**Chapter 3**Carrier Action 2 3 1 4 electron 5 E Carrier Drift • When an electric field (e.g. due to an externally applied voltage) is applied to a semiconductor, mobile charge-carriers will be accelerated by the electrostatic force. • This force superimposes on the random motion of electrons. F=–qE • Electrons drift in the direction opposite to the electric fieldèCurrent flows. • Due to scattering, electrons in a semiconductor do not achieve constant velocity nor acceleration. • However, they can be viewed as particles moving at a constant average drift velocity vd.**Chapter 3**Carrier Action Drift Current vdt All holes this distance back from the normal plane will cross the plane in a time t vdtA All holes in this volume will cross the plane in a time t pvdt A Holes crossing the plane in a time t q pvdt A Charge crossing the plane in a time t qpvd A Charge crossing the plane per unit time I (Ampere) Þ Hole drift current qpvdCurrent density associated with hole drift current J (A/m2)**Chapter 3**Carrier Action Drift Velocity vs. Electric Field • Linear relation holds in low field intensity, ~5103V/cm**Chapter 3**Carrier Action Hole and Electron Mobility has the dimensions ofv/E: Electron and hole mobility of selected intrinsic semiconductors (T = 300 K)**Chapter 3**Carrier Action Hole and Electron Mobility • For holes, • Hole current due to drift • Hole current density due to drift • In low-field limit, • μp : hole mobility • Similarly for electrons, • Electron current density due to drift • μn : electron mobility**Chapter 3**Carrier Action RL RI Temperature Effect on Mobility • Impedance to motion due to lattice scattering: • No doping dependence • Decreases with decreasing temperature • Impedance to motion due to ionized impurity scattering: • Increases with NA or ND • Increases with decreasing temperature**Chapter 3**Carrier Action Temperature Effect on Mobility • Carrier mobility varies with doping: • Decrease with increasing total concentration of ionized dopants. • Carrier mobility varies with temperature: • Decreases with increasing T if lattice scattering is dominant. • Decreases with decreasing T if impurity scattering is dominant.**Chapter 3**Carrier Action Conductivity and Resistivity JN|drift = –qnvd = qnnE JP|drift= qpvd = qppE Jdrift = JN|drift + JP|drift=q(nn+pp)E = E • Conductivity of a semiconductor: =q(nn+pp) • Resistivityof a semiconductor: =1 / **Chapter 3**Carrier Action Resistivity Dependence on Doping • For n-type material: • For p-type material:**Chapter 3**Carrier Action Carrier Mobility as Function Doping Level**Chapter 3**Carrier Action Example • Consider a Si sample at 300 K doped with 1016/cm3 Boron. What is its resistivity? • NA = 1016 cm–3, ND = 0 • (NA >> NDp-type) • p 1016 cm–3, n 104 cm–3**Chapter 3**Carrier Action Example • Consider the same Si sample, doped additionally with 1017/cm3 Arsenic. What is its resistivity now? • NA = 1016 cm–3, ND = 1017 cm–3 • (ND>> NAn-type) • n ND – NA = 9×1016 cm–3, p ni2/n = 1.11×103cm–3**Chapter 3**Carrier Action Example • Consider a Si sample doped with 1017cm–3 As.How will its resistivity change when the temperature is increased from T = 300 K to T = 400 K? • The temperature dependent factor in (and therefore ) is n. • From the mobility vs. temperature curve for 1017cm–3, we find that n decreases from 770 at 300 K to 400 at 400 K. • As a result, increases by a factor of:**Chapter 3**Carrier Action Electron kinetic energy Ec Increasing electron energy Increasing hole energy Ev Hole kinetic energy Potential vs. Kinetic Energy • Ec represents the electron potential energy:**Chapter 3**Carrier Action Band Bending • Until now, Ec and Ev have always been drawn to be independent of the position. • When an electric field E exists inside a material, the band energies become a function of position. E Ec Ev x • Variation of Ec with position is called “band bending”**Chapter 3**Carrier Action Band Bending • The potential energy of a particle with charge –q is related to the electrostatic potential V(x): • Since Ec, Ev, and Ei differ only by an additive constant**Chapter 3**Carrier Action Diffusion • Particles diffuse from regions of higher concentration to regions of lower concentration region, due to random thermal motion (Brownian Motion).**Chapter 3**Carrier Action 1-D Diffusion Example • Thermal motion causes particles to move into an adjacent compartment every τ seconds.**Chapter 3**Carrier Action e- h+ Diffusion Currents n p x x Electron flow Hole flow • D is the diffusion coefficient,[cm2/sec] Current flow Current flow**Chapter 3**Carrier Action Total Currents • Drift current flows when an electric field is applied. • Diffusion current flows when a gradient of carrier concentration exist.**Chapter 3**Carrier Action Current Flow Under Equilibrium Conditions • In equilibrium, there is no net flow of electrons or : • The drift and diffusion current components must balance each other exactly. • A built-in electric field of ionized atoms exists, such that the drift current exactly cancels out the diffusion current due to the concentration gradient.**Chapter 3**Carrier Action Ec(x) EF Ev(x) Current Flow Under Equilibrium Conditions • Consider a piece of non-uniformly doped semiconductor: n-type semiconductor Decreasing donor concentration • Under equilibrium, EF inside a material or a group of materials in intimate contact is not a function of position**Chapter 3**Carrier Action Einstein Relationship between D and m • But, under equilibrium conditions, JN = 0 and JP = 0 Similarly, • Einstein Relationship • Further proof can show thatthe Einstein Relationship is valid for a non-degenerate semiconductor, both in equilibrium and non-equilibrium conditions.**Chapter 3**Carrier Action Example: Diffusion Coefficient • What is the hole diffusion coefficient in a sample of silicon at 300 K with p = 410 cm2 / V.s ? • Remark:kT/q= 25.86 mVat room temperature**Chapter 3**Carrier Action Recombination–Generation • Recombination: a process by which conduction electrons and holes are annihilated in pairs. • Generation: a process by which conduction electrons and holes are created in pairs. • Generation and recombination processes act to change the carrier concentrations, and thereby indirectly affect current flow.**Chapter 3**Carrier Action Generation Processes Band-to-Band R–G Center Impact Ionization Release of energy ET: trap energy level • Due to lattice defects or unintentional impurities • Also called indirect generation EG • Only occurs in the presence of large E**Chapter 3**Carrier Action Recombination Processes Band-to-Band R–G Center Auger Collision • Rate is limited by minority carrier trapping • Primary recombination way for Si • Occurs in heavily doped material**Chapter 3**Carrier Action Homework 2 • 1.(4.17) • Problem 3.6, Pierret’s “Semiconductor Device Fundamentals”. • 2.(4.27) • Problem 3.12, from (a) until (f), for Figure P3.12(a) and Figure P3.12(f),Pierret’s “Semiconductor Device Fundamentals”. • 3.(5.28) • The electron concentration in silicon at T = 300 K is given by • where x is measured in μm and is limited to 0 ≤ x ≤ 25 μm. The electron diffusion coefficient is DN = 25 cm2/s and the electron mobility is μn = 960 cm2/(Vs). The total electron current density through the semiconductor is constant and equal to JN = –40 A/cm2. The electron current has both diffusion and drift current components. • Determine the electric field as a function of x which must exist in the semiconductor. Sketch the function. • Deadline: 1 May 2012, at 14:00 (Tuesday).

More Related